Research Letters in Physics

VolumeΒ 2008, Article IDΒ 786939, 4 pages

http://dx.doi.org/10.1155/2008/786939

## Differential Gain in InGaAsN/GaAs Double Quantum Well Structures by Numerical Simulations

^{1}Department of Physics and Computer Science, Wilfrid Laurier University, Waterloo, ON, Canada N2L 3C5^{2}Department of Physics, Royal Military College, Kingston, ON, Canada K7K 7B4^{3}Institute of Physics, Wroclaw University of Technology, 50-370 Wroclaw, Poland

Received 19 March 2008; Accepted 7 June 2008

Academic Editor: DoerteΒ Blume

Copyright Β© 2008 M. S. Wartak et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

We performed numerical studies of differential gain in a coupled quantum well structures built from InGaAsN. Differential gain in quantum well structures was determined and analyzed. A 10-band Hamiltonian matrix was used in the calculations and solved self-consistently with Poisson's equation. The effect of Nitrogen composition and barrier thickness on differential gain has been determined. The influence of Nitrogen composition on differential gain is significant whereas barrier effects are modest.

#### 1. Introduction

A new material system is currently under intensive investigations. Several properties of those systems have been analyzed [1β3]. is a practical alternative to InP-based materials for operation of quantum-well-based semiconductor lasers. The adventages over InP systems include lower cost, higher characteristic temperature , higher output power, better heat conduction, and applicability to use in vertical cavity surface emitting lasers.

For this new material system there is a need to analyze its properties versus different parameters. One of those parameters is coupling between two quantum wells. Recently, we addressed the question of the effect of well coupling in on the effective masses and optical gain [4, 5]. The optical gain spectra were obtained for various values of Nitrogen composition and barrier widths. They show optimum values for particular barrier width, although the variations are not significant. However, the magnitude of gain peak undergoes significant changes when varying Nitrogen composition.

We have also recently reported on the results of differential gain for single quantum well [6] fabricated using InGaAsN/GaAs material system. It was predicted that spectra of differential gain show significant variation versus Nitrogen composition, well width, and carrier density.

In order to properly manipulate differential gain and optical gain in achieving prescribed engineering goals, we introduced here one more design parameter, namely barrier width of a double-well system. As it is known, for a double quantum well system [7], barrier thickness has a significant effect on differential gain. The differential gain at the gain peak is not a monotonic function of the barrier thickness. For relatively thick barriers inclusion of coupling reduces the differential gain but as the barrier gets thinner the differential gain can be significantly enhanced or suppressed compared to its uncoupled value.

In the present paper, we used the theory leading to the determination of differential gain of two wells consisting of . The details of our approach are described in [5, 6]. The gain formulation incorporates non-Markovian effects, Coulombic interactions, and also band-gap renormalization. In the determination of electron and hole band structures we also incorporated self-consistent effects by solving the relevant matrix Schroedinger equation simultaneously with Poisson's equation.

In Section 2, we outline briefly our formalism and in Section 3 present our results and conclusions.

#### 2. Formalism

The formalism used in our paper has been recently described by us [5]. We use a plane-wave expansion method to calculate the electron and hole bandstructures of the quantum well and a Hamiltonian as presented by TomiΔ et al. [8], where the effect of adding nitrogen to the structure is modeled perturbatively. The Hamiltonian has been also analyzed by OβReilly et al. [9] and Hader et al. [10]. It can be considered as a good model of InGaAsN system. The selection of parameters has been discussed extensively by Choulis et al. [11]. Specific form of this Hamiltonian is Here the subscripts N, C, HH, LH, and SO stand for nitrogen, conduction, heavy-hole, light-hole, and split-off bands, respectively.

The self-consistent method is similar to the one which we used before [12] which consists in a self-consistent solution of the Poisson equation with the matrix Schroedinger equation described by Hamiltonian (1). The Poisson equation is where is the fundamental charge, is the position-dependent permittivity, , and are the position-dependent electron and hole band density distributions, respectively. The function is the electrostatic potential. The density distributions are [12] The symbol represents the conduction (C), heavy-hole (HH) and light-hole (LH) bands and is an index over the subbands. is the conduction band Fermi level and is the valence band Fermi level. Their values are determined by the standard methods [13]. The symbol is Boltzmannβs constant, is temperature, is the average effective mass for the particular band which is approximated as the effective mass in the well since most of the carriers are confined there. Here, and are the respective envelope eigenfunctions and eigenvalues of the various subbands.

We use our previous relation for optical gain quantity [5, 6], which incorporates band-gap renormalization, Coulombic, and non-Markovian effects [14β19]. The TE material gain is given by The details of this equation can be found in [19]. We have added the functional dependence on carrier density for clarity. The term represents the dipole matrix elements for which the calculation of electron and hole wavefunctions was required. For this case, the holes are solved in the LK approximation. The superscript on the variables represents the heavy and light hole bands and and represent the subband indices of the conduction and hole subbands.

The calculations are performed in a self-consistent way as described before [12]. Optical gain is determined using (4). Finally, the differential gain is determined by numerically differentiating expression for TE gain as where is a small increment in the average carrier density in the wells.

#### 3. Results and Conclusions

We performed our analysis for a double quantum well system containing wells and barriers. In our calculations, the well widths are 7βnm and composition of nitrogen in the wells varies from 0.5% to 1.5%. The barrier was varied between 2βnm and 6βnm.

Figure 1 shows differential gain calculated at optical gain peak versus nitrogen composition for several values of barrier thickness. One observes significant dependence of the differential gain on nitrogen composition. For the considered cases, it attains the largest value of for 1.5% of nitrogen, which fits well in the telecommunication window. At the same time, the dependence on the barrier width is relatively weak.

To analyze barrier dependence, in Figure 2 we showed differential gain calculated at optical gain peak versus barrier thickness for several values of nitrogen composition. The strongest dependence on barrier thickness is for 0.5% of nitrogen composition. For 1.5% of nitrogen the value of differential gain for 2βnm to 6βnm barrier's thicknesses is almost flat.

In Figure 3 we analyze spectra of differential gain for the case of 0.5% of nitrogen. The peak of differential gain is around 1080βnm range and shifts towards smaller wavelengths when barrier width increases. It is far from the peak value of optical gain which for 0.5% of nitrogen is around 1190βnm wavelength, see Figure 4. A similar situation can be observed for 1.0% and 1.5% of nitrogen where also peak of differential gain lies in a different range of wavelengths than peak of optical gain.

Finally, in Figure 4 we showed the results of the wavelength dependence of maximum gain and differential gain versus nitrogen composition for 2βnm barrier thickness. One can observe linear dependence of nitrogen composition in both cases. The differential gain spectrum is a direct implication of the conduction band nonparabolicity of GaInNAs alloys which results in the high electron effective mass.

In conclusion, we have analyzed the effects of nitrogen composition and barrier width in a double quantum well system consisting of InGaAsN/GaAs. A 10-band Hamiltonian matrix was used in the calculations and solved self-consistently with Poisson's equation. The effect of nitrogen composition and barrier thickness on differential gain has been determined. The influence of nitrogen composition on differential gain is significant whereas barrier effects are modest.

#### Acknowledgments

The authors would like to acknowledge the support from the Natural Science and Engineering Research Council of Canada (NSERC). This work was made possible by the facilities of the Shared Hierarchical Academic Research Computing Network (SHARCNET: http://www.sharcnet.ca/).

#### References

- M. Kondow, K. Uomi, A. Niwa, T. Kitatani, S. Watahiki, and Y. Yazawa, βGaInNAs: a novel material for long-wavelength-range laser diodes with excellent high-temperature performance,β
*Japanese Journal of Applied Physics*, vol. 35, no. 2, pp. 1273β1275, 1996. View at Google Scholar - M. Kondow and T. Kitatani, βProgress in research into mixed group-V nitride alloys,β
*IEE Proceedings: Optoelectronics*, vol. 150, no. 1, pp. 9β11, 2003. View at Publisher Β· View at Google Scholar - P. J. Klar, βRecent developments in metastable dilute-N III-V semiconductors,β
*Progress in Solid State Chemistry*, vol. 31, no. 4, pp. 301β349, 2003. View at Publisher Β· View at Google Scholar - M. S. Wartak and P. Weetman, βThe effect of well coupling on effective masses in the InGaAsN material system,β
*Journal of Physics: Condensed Matter*, vol. 19, no. 27, Article ID 276202, 8 pages, 2007. View at Publisher Β· View at Google Scholar - M. S. Wartak and P. Weetman, βNumerical studies of optical gain of coupled quantum wells based on InGaAsN material system,β
*Physica Status Solidi (B)*, vol. 245, pp. 726β730, 2008. View at Publisher Β· View at Google Scholar - M. S. Wartak and P. Weetman, βSpectra of differential gain and linewidth enhancement factor in InGaAsN/GaAs
single quantum well structures,β
*Physica Status Solidi (A)*, vol. 204, no. 7, pp. 2487β2494, 2007. View at Publisher Β· View at Google Scholar - A. I. Akhtar and J. M. Xu, βDifferential gain in coupled quantum well lasers,β
*Journal of Applied Physics*, vol. 78, no. 5, pp. 2962β2969, 1995. View at Publisher Β· View at Google Scholar - S. Tomić, E. P. O'Reilly, R. Fehse et al., βTheoretical and experimental analysis of 1.3 $\mu m$ InGaAsN/GaAs lasers,β
*IEEE Journal on Selected Topics in Quantum Electronics*, vol. 9, no. 5, pp. 1228β1238, 2003. View at Publisher Β· View at Google Scholar - E. P. O'Reilly and A. Lindsay, β$k\cdot p$ model of ordered ${\text{GaN}}_{x}{\text{As}}_{1-x}$,β
*Physica Status Solidi (B)*, vol. 216, no. 1, pp. 131β134, 1999. View at Publisher Β· View at Google Scholar - J. Hader, S. W. Koch, J. V. Moloney, and E. P. O'Reilly, βGain in 1.3 $\mu m$ materials: InGaNAs and InGaPAs semiconductor quantum-well lasers,β
*Applied Physics Letters*, vol. 77, no. 5, pp. 630β632, 2000. View at Publisher Β· View at Google Scholar - S. A. Choulis, T. J. C. Hosea, S. Tomić et al., βElectronic structure of ${\text{In}}_{y}{\text{Ga}}_{1-y}{\text{As}}_{1-x}{\text{N}}_{x}/\text{GaAs}$ multiple quantum wells in the dilute-
*N*regime from pressure and $k\cdot p$ studies,β*Physical Review B*, vol. 66, no. 16, Article ID 165321, 9 pages, 2002. View at Publisher Β· View at Google Scholar - P. Weetman, M. S. Wartak, and M. Kucharczyk, βModeling the electrostatic and band-mixing effects on gain for double-quantum-well lasers,β
*Microwave and Optical Technology Letters*, vol. 33, no. 1, pp. 35β37, 2002. View at Publisher Β· View at Google Scholar - S.-L. Chuang,
*Physics of Optoelectronic Devices*, John Wiley & Sons, New York, NY, USA, 1995. - S. Seki, K. Yokoyama, and P. Sotirelis, βTheoretical analysis of high-temperature characteristics of 1.3 $\mu m$ InP-based quantum-well lasers,β
*IEEE Journal on Selected Topics in Quantum Electronics*, vol. 1, no. 2, pp. 264β274, 1995. View at Publisher Β· View at Google Scholar - C.-F. Hsu, P. S. Zory, C.-H. Wu, and M. A. Emanuel, βCoulomb enhancement in InGaAs-GaAs quantum-well lasers,β
*IEEE Journal on Selected Topics in Quantum Electronics*, vol. 3, no. 2, pp. 158β165, 1997. View at Publisher Β· View at Google Scholar - M. J. Connelly, βWideband semiconductor optical amplifier steady-state numerical model,β
*IEEE Journal of Quantum Electronics*, vol. 37, no. 3, pp. 439β447, 2001. View at Publisher Β· View at Google Scholar - W. W. Chow, S. W. Koch, and M. Sargent III,
*Semiconductor-Laser Physics*, Springer, Berlin, Germany, 1997. - J. Minch, S. H. Park, T. Keating, and S. L. Chuang, βTheory and experiment of ${\text{In}}_{1-x}{\text{Ga}}_{x}{\text{As}}_{y}{\text{P}}_{1-y}$ and ${\text{In}}_{1-x-y}{\text{Ga}}_{x}{\text{Al}}_{y}\text{As}$ long-wavelength strained quantum-well lasers,β
*IEEE Journal of Quantum Electronics*, vol. 35, no. 5, pp. 771β782, 1999. View at Publisher Β· View at Google Scholar - D. Ahn, βOptical gain of a quantum-well laser with non-Markovian relaxation and many-body effects,β
*IEEE Journal of Quantum Electronics*, vol. 32, no. 6, pp. 960β965, 1996. View at Publisher Β· View at Google Scholar